We can conduct ASTM G61 for selection of materials in highly corrosive environments. ASTM provides the following :
Significance and Use
3.1 An indication of the susceptibility to initiation of localized corrosion in this test method is given by the potential at which the anodic current increases rapidly. The more noble this potential, obtained at a fixed scan rate in this test, the less susceptible is the alloy to initiation of localized corrosion. The results of this test are not intended to correlate in a quantitative manner with the rate of propagation that one might observe in service when localized corrosion occurs.
3.2 In general, once initiated, localized corrosion can propagate at some potential more electropositive than that at which the hysteresis loop is completed. In this test method, the potential at which the hysteresis loop is completed is determined at a fixed scan rate. In these cases, the more electropositive the potential at which the hysteresis loop is completed the less likely it is that localized corrosion will occur.
3.3 If followed, this test method will provide cyclic potentiodynamic anodic polarization measurements that will reproduce data developed at other times in other laboratories using this test method for the two specified alloys discussed in 3.4. The procedure is used for iron-, nickel-, or cobalt-based alloys in a chloride environment.
3.4 A standard potentiodynamic polarization plot is included. These reference data are based on the results from five different laboratories that followed the standard procedure, using specific alloys of Type 304 stainless steel, UNS S30400 and Alloy C-276, UNS N10276.3 Curves are included which have been constructed using statistical analysis to indicate the acceptable range of polarization curves.
3.5 The availability of a standard test method, standard material, and standard plots should make it easy for an investigator to check his techniques to evaluate susceptibility to localized corrosion.
1.1 This test method covers a procedure for conducting cyclic potentiodynamic polarization measurements to determine relative susceptibility to localized corrosion (pitting and crevice corrosion) for iron-, nickel-, or cobalt-based alloys in a chloride environment. This test method also describes an experimental procedure which can be used to check one’s experimental technique and instrumentation.
Potential vs Current Density plot to determine relative susceptibility to localized corrosion in sea water
We are here to help
We respond to all customers promptly by sending a technical proposal to address testing, investigation and the proposal costs. If we need more information, our engineers will contact you.We respond to all customers promptly by sending a technical proposal to address testing, investigation and the proposal costs. If we need more information, our engineers will contact you. Whether you are a large corporation or a small enterprise, we will provide you with the attention you need and deserve. In so doing, we hope to work with you for many years to come.
Please call Dr. Zee at 412-952-9441 and let us know how we can assist you in your investigation. Alternatively, you can send your request to email@example.com.
Looking forward to hearing from you!